USING STANDARD PRB SPHYSICAL REVIEW B 15 SEPTEMBER 1999-IVOLUME 60,
Reinterpretation of the scanning tunneling microscopy images of
Kenji Hata,* Satoshi Yasuda, and Hidemi Shigekawa* Institute of
Applied Physics and CREST, Japan Science and Technology Corporation
(JST), University of Tsukuba,
Tennodai 1-1-1, Tsukuba 305-8573, Japan ~Received 4 May 1998;
revised manuscript received 1 April 1999!
We revisit and refine the interpretation of the scanning tunneling
microscopy~STM! images of the Si~100! dimers, based on results from
an extensive set of STM observations carried out at low
temperature~80 K! and total-energy calculations of Si~100!
surfaces. The interpretation addresses some unresolved questions
and brings much experimental and theoretical research into
unanimous agreement. We show that tunneling from surface resonances
and bulk states seriously contributes to the STM images within
usual tunneling conditions. In the empty state, tunneling from
these states overwhelms tunneling from the localizedp* surface
state, which STM is generally believed to
e r p
le ges the e u-
ar ate how the d le as ace led ip- all ob- f -
Even though the dimer of Si~100! is one of the most simple surface
reconstructions, it has turned out to b source of neverending
controversy. A great deal of resea has been devoted to elucidate
its atomic configuration, o cal properties, and electronic
structure.1–6 In particular, scan- ning tunneling microscopy~STM!
has considerably contrib uted to enlighten our understandings.1–6
Generally, it is interpreted that STM observes the surface states
localize the dangling bonds of the dimers.1,2 Interpretation of the
STM images of the dimers from this standpoint seems to simple and
in accordance with what is expected from general laws of chemical
bonding.1 However a careful analy sis of the existing data reveals
that our understanding is complete, and in the following we point
out two problem which require further consideration.
The first question is concerned with the interpretation the
filled-state STM images obtained at room temperature to now.
Previous room-temperature STM studies sh dimers as bean-shaped
protrusions which have a maxim at the center of the Si-Si dimer
bond in the filled states.1,2 We nominate them as bean-type dimers
in the following. In c trast, when the empty states are probed, two
round sh protrusions are resolved,2 which we refer to as protrusion
type dimers. These STM images are easily explained by suming
symmetric dimers,1 though it is now well established that dimers
are buckled.3 Indeed at temperatures below;200 K ~low
temperatures!, a majority of the dimers is observed i a buckled
configuration.3 Buckling induces a charge transfe from the lower to
upper atom of the dimer, and the filledp and emptyp* surface states
are localized at the dangl bonds of the upper and lower atoms of
the buckled dim respectively. Generally, it is assumed that thep
andp* sur- face states1,2 are observed in the STM images as dimers.
order to interpret the apparent symmetric dimers observe STM at
room temperature within the framework of buckl dimers, the concept
of flip-flop motion was introduced: buc led dimers are
flip-flopping far faster than the scanning STM, thus dimers appear
in an apparent symmetric confi ration. In this scheme, STM images
obtained at room te perature must reflect the average of STM images
of the bu
- f u- - k-
led dimers at low temperature in the two possib configurations. It
is easy to interpret the empty-state ima at room temperature: the
two protrusions observed in (231) unit cell are both thep* surface
state localized at th lower atom of the buckled dimer in the two
possible config rations. On the other hand, it is puzzling why
simil protrusion-type dimers are not observed in the filled st
instead of the bean-shaped dimers. Indeed, in Fig. 1 we s gray
scale images of the simulated spatial distribution of flip-flopped
filledp and emptyp* surface states calculate by first-principle
methods. Methodology of the first-princip calculations is presented
in Sec. III C. Flip-flop motion w simulated by adding the
electronic structure of the surf states in the two possible
configurations of the buck dimer. It is a surprise to notice that
the images of the fl floppedp andp* surface states are very similar
with a sm node in between the dimer. A similar result has been
tained by Owenet al., where they simulated STM images o the
flip-flopping buckled dimers following Tersoff and Ham man’s
formalism. Their simulation shows a protrusion-ty STM image of the
dimers in the filled [email protected]
. 2~a! in Ref. 7#.
The second problem is the mismatch between the typ surface bias
used to observe the surface in the past and energy window where
thep andp* surface states are loca ized. A survey of previous STM
observations of the Si~100!
FIG. 1. Cross sections of the electronic and atomic structure the
simulated flip-flopped buckled dimers.~a! Simulated filledp surface
state and~b! p* empty surface state. Cross sections we taken along
a plane which includes the buckled dimer. The sm black and large
gray circles represent the position of the upper lower atom of the
buckled dimer, respectively. The electronic str ture was calculated
by first-principles methods and the flip-flop m tion was simulated
by adding the two possible configurations.
8164 ©1999 The American Physical Society
flip- bi- is ow
PRB 60 8165REINTERPRETATION OF THE SCANNING TUNNELING . . .
surface reveals that most of the STM images are of the fi states
taken with a surface bias as large as22 V.1–5 How- ever, the
typical bias of22 V is out of the range of where thep surface state
is located. We can see this by conside the surface band gap and the
width of the surface sta Typical I -V curves of the dimers show a
surface band gap ;0.5 V with the Fermi level located in the
midgap.4 The surface band gap of;0.5 V is also supported from othe
experiments.8 Theoretical9 and photoemission10,11 studies show that
the bandwidths of thep andp* states are 0.6–0.8 V each. When
combined with the surface band gap of;0.5 V, this means that thep
and p* surface states are rough localized in the range of;61 V from
the Fermi level. In a typical STM image taken at22 V, a significant
part of the tunneling current must come from states other than the
facep andp* states.
In this paper, we provide results from an extensive se STM
observations at room and low temperature~80 K!, and present a
refined interpretation of the STM images of dim In our
interpretation, at typical tunneling conditions used the past, a
serious part of the tunneling current comes f states other than
thep andp* surface states. The new inte pretation addresses the
aforementioned unresolved ques and brings results of much
experimental and theoretical search into unanimous agreement.
Defects are the major reason why high biases~;22 V! were used in
the past. It is believed that surfaces of Si~001! inevitably
contain a significant density of defects. When o attempts to lower
the bias, these defects become very b because many defects are
metallic, making it difficult to o serve the dimers clearly. We
have overcome this problem fabricating a surface with very low
defect density. After t sample was prebaked at;700 °C for one
night, it was flashed to 1200 °C for several seconds. The pressure
kept below 131028 Pa during flashing~in most times around 531029
Pa). We found that keeping this extreme good vacuum pressure during
flashing is crucial to hav surface with low defect density.12 By
this procedure, a clean Si~100! surface with a small ratio of
defects lower than 0.2 was repeatedly made on any provided
sample.N-type Si samples phosphorus-doped with a conductivity of
0.1V cm were used. TunnelingI -V measurements of the surface sho
that the Fermi level is at the upper edge of the conduc band, which
agrees with then-type doping, and a width o the surface band gap
III. RESULTS AND DISCUSSION
A. STM results at room temperature
Surfaces free from defects make observation of the dim possible at
any desired surface bias. Figure 2~a! shows an STM image of the
filled state probed with a low surface b just below the surface
band gap~20.6 V! at room tempera- ture. Not a bean-type but a
protrusion-type dimer is o served. We could observe the
protrusion-type dimers in filled states at low surface biases with
the same frequenc in the empty state. The protrusions are observed
at the s location where the empty-state protrusions are
- e as me us
we attribute them to be observing thep surface state located at the
dangling bond of the upper atom of the dimer. Ev time the bias is
increased, the dimers would gradually rev to the bean type at;21 V
as shown in Fig. 2~b!, in a reversible fashion. This indicates that
the protrusion-ty dimers observed here are not induced by some
peculiar surface interaction.
The empty-state STM images show a more complica dependence on bias.
When the surface bias is above11.4 V, regions between the dimer
rows are observed. This is h lighted in Fig. 2~c!, where the bias
was switched from a lo ~0.6 V! to a high bias~1.5 V! in the
intermediate of scanning Immediately it is apparent that the bright
rows observed low ~0.6 V! and high biases~1.5 V! are completely out
of phase. We attribute the bright rows observed at low biase the
dimers, since they are in-phase with the dimer rows served in the
filled state. This means that regions between dimers are observed
at high biases. The phase shift occu a bias around 1.4 V. The phase
shift was repor previously1 and was interpreted as an extension of
the no of the antibonding state of a symmetric dimer with bi which
was lately supported by theoretical studies.13 How- ever, as
mentioned before, dimers are buckled, and thep* surface state of
buckled dimers is calculated not to sh such an extension with
bias.13 Considering these points, w interpret that at high biases,
the main part of the tunnel current comes from states localized
between the dimer ro overwhelming tunneling from thep* surface
Results obtained at room temperature are summari Protrusion-type
dimers are observed both in the empty filled states at low biases.
On the other hand, at high bia bean-type dimers are observed in the
filled states while region between the dimer rows is observed in
the em states. We interpret the results as the following.~i! At low
biases, STM observes thep or p* surface states. The protrusion-type
dimers are observed as a result of the flop motion of the buckled
dimers. The range of surface ases~21 V to ;11.4 V! where the
protrusion-type dimers observed is in good accordance with the
energy wind where thep andp* bands are localized.~ii ! At high
FIG. 2. STM images of dimers at room temperature.~a! Low bias
filled state~20.6 V!. ~b! The bias was gradually decrease from 20.9
to 21.7 V. The bean⇔protrusion transition of the dimers occurred
around;21 V. The reason why the bean-shape dimers are not clearly
visible at high biases might be because image was taken
simultaneously with the protrusion-type dim observed at low biases,
which show stronger contrast than the b type dimers.~c! Empty-state
image. The surface bias was switch from a low ~10.6 V! to a
high~11.5 V! bias in the middle.
8166 PRB 60KENJI HATA, SATOSHI YASUDA, AND HIDEMI SHIGEKAWA
tunneling from other states starts to participate in, and in empty
states overwhelm, tunneling from thep* surface state. The spatial
distribution of the other states is locali between the Si-Si dimer
bond in the filled states and betw the dimer rows in the empty
states, respectively. The n STM images and interpretation presented
here address two problems mentioned in the Introduction. Moreov
many experimental results—the widths of thep and p* bands, surface
band gap obtained fromI -V curves, and the voltage dependence of
the STM images—come into s coincidence within the familiar notion
of flip-flopping buck led dimers.
B. STM results at low temperature „80 K…
In order to reinforce our assertions, an extensive se STM
observations was carried out at a low temperature~80 K! where the
flip-flop motion of dimers is frozen. We sho that the
low-temperature STM images of the dimers una mously coincide with
the complementary room-temperat results further supporting our
First we provide results of the observation of the fill states.
Figure 3 shows some typical filled-state STM ima of the dimers with
different biases ranging from20.8 to 22.0 V to show the dependence
of the STM images on s face bias. STM images taken at low
bias~;21.0 V! show clear zigzag chains forming ac(432) phase,3
which we interpret to reflect tunneling from thep surface state
local ized at the upper atom of the dimer. The upper atom of dimers
and the dimer rows are aligned in an antiferrom netic order
providing the observedc(432) phase. Based on this understanding,
the locations of the upper atoms of dimers are assigned as black
circles in the STM image ta at 20.8 V. As the bias is increased,
thec(432) zigzag component fades and instead a (231) component
emerge and grows in intensity as shown in the STM images
FIG. 3. STM images~1 nA! of the filled states of the dimers a
surface biases ranging from20.8 to 22.0 V at 80 K. Scale 434
high biases above21.5 V. At 22 V, the STM image re- sembles ac(432)
zigzag component overlapped with (231) component. In order to
investigate this fading effe more quantitatively, average cross
sections of the dimer the STM images taken at high~22.0 V! and low
~20.8 V! biases are shown in Figs. 4~a! and 4~b!, respectively.
Cross sections are taken at the locations displayed as dashed b in
Fig. 3. In addition, we display the cross section of t electronic
structure of thep surface state calculated by firs principle
methods in Fig. 4~c! for comparison. We registere Fig. 4~c! against
Figs. 4~a! and 4~b! by attributing the global minimum of the cross
sections to the middle of the dim rows where the lower atoms of the
dimers are at the adjac By comparing Figs. 4~b! and 4~c!, we can
understand tha STM is not observing the atoms of the dimers and the
c rugation in the STM images reflects the global corrugation the
electronic structure with some diminished spatial reso tion. From
Fig. 4~b!, it is apparent that there exists two type of minima
aligned alternatively in the cross sections. Minim A and B defined
in Fig. 4 are both located in the midd between the dimers, though
they are different because upper~lower! atoms are located at the
immediate adjacen minimumA (B). This difference is due to the34
periodic- ity of the reconstruction in this direction and gradually
d creases as the bias is increased as shown in Fig. 4~a!. We define
the height difference between the two minimaA andB
FIG. 4. Average cross section of the filled-state STM imag taken
at~a! a high bias~22.0 V! and ~b! a low bias~20.8 V!. ~c! Cross
section of the electronic structure of the filledp surface state.
Two types of minima indicated byA and B in the cross sections exist
aligned alternatively. HD is defined as the height differen
betweenA andB, and Corr as the average corrugation of the dime ~d!
Dependence of HD/Corr on surface bias. Also HD vs surfa bias is
displayed in the inset.
PRB 60 8167REINTERPRETATION OF THE SCANNING TUNNELING . . .
as HD, and the average corrugation of the dimers as Co shown in
Figs. 4~a! and 4~b!. HD divided by the corrugation of the
dimers~Corr! is assumed to serve as an indicator the strength of
thec(432) zigzag component versus th (231) component. The
dependence of HD/Corr on the s face bias is plotted in Fig. 4~d!.
Also HD versus surface bia is displayed in the inset of Fig. 4~d!.
HD/Corr remains con- stant below21.4 V and gradually decreases with
increas biases. It should be noted that even at biases as high a22
V, HD/Corr does not drop to zero, thus the remaini c(432) zigzag
component should have been observed reported as buckled dimers in
previous studies.3,14–16We in- terpret the experimental results as
the following.~i! Tunnel- ing from thep surface state is observed
at low biases n the Fermi edge.~ii ! A decrease of thec(432) zigzag
com- ponent at high bias reflects an opening of a new tunne channel
from other states which are mainly localized in tween the Si-Si
dimer bond and have an almost (231) pe- riodicity. ~iii ! As the
bias is increased, tunneling from oth states becomes important and
thec(432) zigzag componen fades. Tunneling from the other states at
high biases sh be the cause of the protrusion⇔bean-type transitions
of th appearance of the dimers observed in the filled states at r
Next, we shift to the observations of the empty states low
temperature. Figure 5 shows an STM image at low te perature~80 K!
where the bias was switched from a low~0.6 V! to a high bias~1.5 V!
in the intermediate. Again, the phase shift is observed, and areas
between the dimer are observed at the high bias. Dimers appear
different in STM images taken at low and high biases. At the low bi
STM images show rows of zigzag chains in ac(432) phase,3 which
reflects tunneling from thep* surface state localized at the lower
atom of the dimer. In contrast, at high bias, a bright row similar
to that observed at room te perature is obtained, though a bright
and dark (231) unit
FIG. 5. An STM image~1 nA! of the empty states at 80 K.~a! The bias
was switched from a low~0.6 V! to a high~1.5 V! bias in the
align alternatively along the dimer-row direction. Th brighter
units are registered against thec(432) region scanned with low
bias, from which we attribute the low atom of the dimer to a circle
as shown in Fig. 5. It shows t the brighter unit corresponds to the
location of the up atom of the dimer. This cannot be explained by
an extens of the wave function of thep* state localized at the lowe
atom with bias, but means that tunneling from other sta becomes
important at high biases. In order to investigate details of the
phase shift with bias, we have carried out S observations of the
dimers on a defect-freec(432) buckled dimer domain scanned with
different biases ranging from to 2.1 V with an increase rate of 0.1
V as shown in Fig. Also a set of cross sections of the STM images
of Fig along the dimers are displayed in Fig. 7. In the lower sect
of Fig. 7, the cross section of the calculated electronic str ture
of thep* surface state is displayed for clarity. Regist was done in
the same fashion employed to display Fig. 4~c!. The same phase
shift presented in Fig. 5 is evident. At biases below 1.4 V, two
types of minima in the cross s tions are clearly observable, which
reflects thec(432) zig- zag component, likewise the case of the
observations of filled states. We interpret that tunneling from
thep* surface state localized at the lower atom of the dimer is
observed these low biases. As the bias increases and approaches 1
the corrugations of the dimers gradually decrease, wh should
reflect an opening of tunneling channels from ot states. It is a
surprise to observe an almost flat STM imag the transition bias of
1.4 V. As the bias is increased ab
FIG. 6. STM images of the empty states at surface biases r ing from
0.8 to 1.9 V at 80 K. Tunneling current 0.6 nA. Sca 535 nm.
8168 PRB 60KENJI HATA, SATOSHI YASUDA, AND HIDEMI SHIGEKAWA
1.4 V, a new corrugation emerges which is out of phase w that
observed at low biases. The new corrugation observe high biases is
characterized by two types of maxima alig alternatively forming a34
periodicity in contrast to the two types of minima observed at low
biases. Again, the lo temperature results are fully consistent with
the roo temperature observations.
Subsequently, we register the filled-state STM imag against the
empty-state images taken at low biases to em size their similarity
and to show that band bending does affect our interpretation.
Figure 8 shows an STM image the dimers at low temperature~80 K!
where the bias was switched from positive to negative in the
intermediate scanning at the location indicated by the black line.
Hen the upper half is an empty-state image while the lower ha an
image of the filled state both taken at low biases. Si larity
between the dimers in the STM images of the em and filled states is
striking, which agrees with the protrusi type image of dimers
obtained at room temperature both the empty and filled states at
low biases. Moreover, wha more important is that the opposite side
of the dimer is
FIG. 7. Cross section of STM images of Fig. 6 along the dime The
inset in the bottom shows the cross section of the electr structure
of thep* surface state.
h at d
s i- y - in is -
served in the empty and filled states. This is emphasized matching
ac(432) phased stick and ball pattern to th c(432) zigzag component
of the STM image. Obvious the stick and ball patterns observed in
the empty and fi states are out of phase, giving other evidence
that thep and p* surface states localized at the opposite side of
the di are observed in the STM images taken at low biases. F
FIG. 8. An STM image~1 nA! showing both the filled and empty states
at 80 K. The bias was switched from positive~10.6 V! to
negative~20.8 V! in the intermediate of scanning at the locatio of
the black line. The stick and ball schematics are assigned to
c(432) zigzag components of the STM image, which reflect tu neling
from thep* andp surface states.
FIG. 9. Spatial distribution of the electronic density of states
the buckled dimers within62 V of the Fermi energy except thep andp*
bands.~a! Filled states.~b! Empty states.D andU indicate the lower
and upper atoms of the buckled dimer, respectively.
TM te d ob s s
e g en n di
at m e rg
m - th
PRB 60 8169REINTERPRETATION OF THE SCANNING TUNNELING . . .
thermore, we can definitely state that the filled-state S images
taken at low bias are really observing the filled sta not the empty
states. This is important because it exclu the possibility that the
appearance of protrusion dimers served at room temperature in the
filled states at low biase due to observing the empty states at
negative surface bia a result of band bending.
Variation of the tip-surface distance with bias is anoth possible
explanation for the dependence of the STM ima on bias. All of the
STM images in Figs. 3 and 6 were tak at a constant current, thus an
increase in bias means a crease in the tunneling barrier height and
the tip-surface tance. Generally, an increase in the tip-surface
distance sults in a decrease of resolution, which one might suspec
be the cause of the protrustion⇔bean ~room-temperature!,
zigzag⇔bean transitions~low temperature! of the appear- ance of the
dimers observed in the filled states. However this mechanism the
phase shift observed in the empty s cannot be explained.
Furthermore, STM images taken at stant barrier height (13109 V)
also show an identical tran sition shown in Figs. 3 and 6 at the
same bias in the sa fashion. Strictly speaking, constant barrier
height does mean a constant tip-surface distance. Since the feedbac
STM is regulated to keep the tunneling current constant particular
bias, it is difficult to scan the surface with the sa tip-surface
distance at different biases. Considering th factors, we have
compared STM images taken with a la barrier height~far from the
surface! at low biases~21 V, 100 pA! and with a small barrier
height~close to the surface! at high biases~22 V, 64 nA!. The STM
images were basicall the same, though somewhat of an increase of
the zigzag chain component was observed at high bias. We did not
serve complete zigzag chained dimers at high biases, thu rule out
the variation of tip-surface distance as the m cause of the
dependence of STM images on bias.
C. Theoretical calculations
STM observations consistently show that tunneling fro states other
than thep and p* surface states becomes im portant at high biases.
In this section we briefly discuss possible states observed at high
biases. As thep andp* are the only localized surface states of the
buckled dimers, have to consider the more extended surface
resonances the bulk continuum states. We refer to the calculations
c ried out by Krugeret al.,17,18 where they have employed
self-scattering theoretical method based on first princip which is
suited to calculate surface resonances extendi long range into the
bulk. In their calculations, the back bo (B1) and dimer bond (D1
,Di* ) states were shown to lie close to thep andp* surface states
in energy~look at Fig. 5 in Ref. 18!. We assign them as the states
observed by S at high voltages.
s, es - is as
In order to give a rough idea of the spatial distributions these
states, the spatial distribution of overlapped ba within 62 V of
the Fermi energy in the filled and empt states, except thep andp*
bands, was calculated. Standar formalism of first-principle
calculations was employed wit the local-density approximation and
plane-wave-based n local pseudopotentials with a cutoff energy of
10 Ry. Calc lations were carried out on ac(432) supercell
containing a slab of silicon ten layers thick geometrically
optimized b Ramstad9 with a vacuum region of five layers thickness.
must be noted that the supercell technique is not suited treat
surface resonances which extend into the bulk. Hen in this paper,
the aim of our calculation is to roughly es mate whether or not the
spatial distribution of bands loca near to the Fermi energy, except
thep and p* bands, is similar to what was observed in the STM
images at hi biases. Figure 9 shows the spatial distribution of
states n the Fermi energy except thep and p* bands. A strong in-
tensity in the middle of the Si-Si dimer bond in the fille
. 9~a!# is observed, while they are localized mainl
between the dimer rows in the empty [email protected]
. 9~b!#, in
coincidence with the STM observations. In order to give more
detailed analysis, we have to calculate the surface re nances with
a more proper method or use a very deep ce which the effect of the
thickness of the cell becomes neg gible. Also we have to simulate
the STM images by comb ing the calculated electronic structures
with the tunneli probabilities. Matching STM images and theoretical
calcu tions would be an interesting subject for future work.
This study has two important implications for future STM studies on
Si~100!. First, careful attention must be paid whe one observes the
empty states and attempts to investigate locations of absorbates;
if the surface is probed at high bia unintentionally one would make
an erroneous attributio Also, it is important to use a low surface
bias when obse ing the filled states, particularly when studying
absorbates some extreme cases we have observed a surface which m
ics a perfect surface at22 V, but shows many defects at21 V. These
defects might influence the sites of adsorption the electronic
characteristics. If the absorbates only influe the p and p* states,
they might be even invisible at hig biases.
This work was supported by the Shigekawa Project TARA, University
of Tsukuba. The support of a Grant-in Aid for Scientific Research
from the Ministry of Education Science and Culture of Japan is also
*Electronic address: [email protected]
firstname.lastname@example.org World Wide Web:
1R. J. Hamers, R. M. Tromp, and J. E. Demuth, Phys. Rev. B34, 5343
2R. J. Hamers, Ph. Avouris, and F. Bozso, Phys. Rev. Lett.59,
2071 ~1987!. 3R. A. Wolkow, Phys. Rev. Lett.68, 2636~1992!. 4A. W.
Munz, Ch. Ziegler, and W. Gopel, Phys. Rev. Lett.74,
2244 ~1995!. 5H. Shigekawa, K. Hata, K. Miyake, M. Ishida, and S.
Phys. Rev. B55, 15 448~1997!.
8170 PRB 60KENJI HATA, SATOSHI YASUDA, AND HIDEMI SHIGEKAWA
6K. Hata, M. Ishida, K. Miyake, and H. Shigekawa, Appl. Phy Lett.
73, 40 ~1998!.
7J. H. G. Owen, D. R. Bowler, C. M. Goringe, K. Miki, and G. A D.
Broggs, Surf. Sci.341, L1042 ~1995!.
8Y. J. Chabal, S. B. Christmann, E. E. Chaban, and M. T. Yin Vac.
Sci. Technol. A1, 1241~1983!.
9R. Ramstad, G. Brocks, and P. J. Kelly, Phys. Rev. B51, 14 504
10Y. Enta, S. Suzuki, and S. Kono, Phys. Rev. Lett.65, 2704
12K. Hata ~unpublished!. 13H. Kageshima and M. Tsukada, Phys. Rev.
B46, 6928~1992!. 14H. Tochihara, T. Amakusa, and M. Iwatsuki, Phys.
12 262~1994!. 15D. Badt, H. Wengelnik, and H. Neddermeyer, J. Vac.
nol. B 12, 2015~1994!. 16A. R. Smith, F. K. Men, K.-J. Chao, and C.
K. Shih, J. Vac. S
Technol. B14, 914 ~1996!. 17P. Kruger, A. Mazur, J. Pollmann, and
G. Wolfgarten, Phys. R